LMucko/crystallography-open-database huggingface dataset:
X-ray measurement of the thermal expansion of pure nickel Sample: at T = 398 C Note: film 556
Owen, E. A.; Yates, E. L.; Philosophical Magazine 21 (1936) 809–819; doi:

data_9012996
_publ_section_title
;
 X-ray measurement of the thermal expansion of pure nickel
 Sample: at T = 398 C
 Note: film 556
;
_journal_name_full               'Philosophical Magazine'
_journal_page_first              809
_journal_page_last               819
_journal_volume                  21
_journal_year                    1936
_chemical_compound_source        Synthetic
_chemical_formula_sum            Ni
_chemical_name_mineral           Nickel
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.5383
_cell_length_b                   3.5383
_cell_length_c                   3.5383
_cell_formula_units_Z            4
_cell_volume                     44.298
_database_code_amcsd             0014986
_diffrn_ambient_temperature      671.15
_exptl_crystal_density_diffrn    8.800
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9012996
X-ray measurement of the thermal expansion of pure nickel Sample: at T = 405 C Note: film 613
Owen, E. A.; Yates, E. L.; Philosophical Magazine 21 (1936) 809–819; doi:

data_9012997
_publ_section_title
;
 X-ray measurement of the thermal expansion of pure nickel
 Sample: at T = 405 C
 Note: film 613
;
_journal_name_full               'Philosophical Magazine'
_journal_page_first              809
_journal_page_last               819
_journal_volume                  21
_journal_year                    1936
_chemical_compound_source        Synthetic
_chemical_formula_sum            Ni
_chemical_name_mineral           Nickel
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.5386
_cell_length_b                   3.5386
_cell_length_c                   3.5386
_cell_formula_units_Z            4
_cell_volume                     44.309
_database_code_amcsd             0014987
_diffrn_ambient_temperature      678.15
_exptl_crystal_density_diffrn    8.798
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9012997
X-ray measurement of the thermal expansion of pure nickel Sample: at T = 410 C Note: film 607
Owen, E. A.; Yates, E. L.; Philosophical Magazine 21 (1936) 809–819; doi:

data_9012998
_publ_section_title
;
 X-ray measurement of the thermal expansion of pure nickel
 Sample: at T = 410 C
 Note: film 607
;
_journal_name_full               'Philosophical Magazine'
_journal_page_first              809
_journal_page_last               819
_journal_volume                  21
_journal_year                    1936
_chemical_compound_source        Synthetic
_chemical_formula_sum            Ni
_chemical_name_mineral           Nickel
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.5388
_cell_length_b                   3.5388
_cell_length_c                   3.5388
_cell_formula_units_Z            4
_cell_volume                     44.317
_database_code_amcsd             0014988
_diffrn_ambient_temperature      683.15
_exptl_crystal_density_diffrn    8.796
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9012998
X-ray measurement of the thermal expansion of pure nickel Sample at T = 411 C Note: film 609
Owen, E. A.; Yates, E. L.; Philosophical Magazine 21 (1936) 809–819; doi:

data_9012999
_publ_section_title
;
 X-ray measurement of the thermal expansion of pure nickel
 Sample at T = 411 C
 Note: film 609
;
_journal_name_full               'Philosophical Magazine'
_journal_page_first              809
_journal_page_last               819
_journal_volume                  21
_journal_year                    1936
_chemical_compound_source        Synthetic
_chemical_formula_sum            Ni
_chemical_name_mineral           Nickel
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.5388
_cell_length_b                   3.5388
_cell_length_c                   3.5388
_cell_formula_units_Z            4
_cell_volume                     44.317
_database_code_amcsd             0014989
_diffrn_ambient_temperature      684.15
_exptl_crystal_density_diffrn    8.796
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9012999
X-ray measurement of the thermal expansion of pure nickel Sample: at T = 429 C Note: film 591
Owen, E. A.; Yates, E. L.; Philosophical Magazine 21 (1936) 809–819; doi:

data_9013000
_publ_section_title
;
 X-ray measurement of the thermal expansion of pure nickel
 Sample: at T = 429 C
 Note: film 591
;
_journal_name_full               'Philosophical Magazine'
_journal_page_first              809
_journal_page_last               819
_journal_volume                  21
_journal_year                    1936
_chemical_compound_source        Synthetic
_chemical_formula_sum            Ni
_chemical_name_mineral           Nickel
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.5402
_cell_length_b                   3.5402
_cell_length_c                   3.5402
_cell_formula_units_Z            4
_cell_volume                     44.369
_database_code_amcsd             0014990
_diffrn_ambient_temperature      702.15
_exptl_crystal_density_diffrn    8.786
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9013000
X-ray measurement of the thermal expansion of pure nickel Sample: at T = 460 C Note: film 572
Owen, E. A.; Yates, E. L.; Philosophical Magazine 21 (1936) 809–819; doi:

data_9013001
_publ_section_title
;
 X-ray measurement of the thermal expansion of pure nickel
 Sample: at T = 460 C
 Note: film 572
;
_journal_name_full               'Philosophical Magazine'
_journal_page_first              809
_journal_page_last               819
_journal_volume                  21
_journal_year                    1936
_chemical_compound_source        Synthetic
_chemical_formula_sum            Ni
_chemical_name_mineral           Nickel
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.5422
_cell_length_b                   3.5422
_cell_length_c                   3.5422
_cell_formula_units_Z            4
_cell_volume                     44.445
_database_code_amcsd             0014991
_diffrn_ambient_temperature      733.15
_exptl_crystal_density_diffrn    8.771
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9013001
X-ray measurement of the thermal expansion of pure nickel Sample: at T = 501 C Note: film 561
Owen, E. A.; Yates, E. L.; Philosophical Magazine 21 (1936) 809–819; doi:

data_9013002
_publ_section_title
;
 X-ray measurement of the thermal expansion of pure nickel
 Sample: at T = 501 C
 Note: film 561
;
_journal_name_full               'Philosophical Magazine'
_journal_page_first              809
_journal_page_last               819
_journal_volume                  21
_journal_year                    1936
_chemical_compound_source        Synthetic
_chemical_formula_sum            Ni
_chemical_name_mineral           Nickel
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.5448
_cell_length_b                   3.5448
_cell_length_c                   3.5448
_cell_formula_units_Z            4
_cell_volume                     44.543
_database_code_amcsd             0014992
_diffrn_ambient_temperature      774.15
_exptl_crystal_density_diffrn    8.752
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9013002
X-ray measurement of the thermal expansion of pure nickel Sample: at T = 557 C Note: film 575
Owen, E. A.; Yates, E. L.; Philosophical Magazine 21 (1936) 809–819; doi:

data_9013003
_publ_section_title
;
 X-ray measurement of the thermal expansion of pure nickel
 Sample: at T = 557 C
 Note: film 575
;
_journal_name_full               'Philosophical Magazine'
_journal_page_first              809
_journal_page_last               819
_journal_volume                  21
_journal_year                    1936
_chemical_compound_source        Synthetic
_chemical_formula_sum            Ni
_chemical_name_mineral           Nickel
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.5481
_cell_length_b                   3.5481
_cell_length_c                   3.5481
_cell_formula_units_Z            4
_cell_volume                     44.667
_database_code_amcsd             0014993
_diffrn_ambient_temperature      830.15
_exptl_crystal_density_diffrn    8.727
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9013003
X-ray measurement of the thermal expansion of pure nickel Sample: at T = 603 C Note: film 568
Owen, E. A.; Yates, E. L.; Philosophical Magazine 21 (1936) 809–819; doi:

data_9013004
_publ_section_title
;
 X-ray measurement of the thermal expansion of pure nickel
 Sample: at T = 603 C
 Note: film 568
;
_journal_name_full               'Philosophical Magazine'
_journal_page_first              809
_journal_page_last               819
_journal_volume                  21
_journal_year                    1936
_chemical_compound_source        Synthetic
_chemical_formula_sum            Ni
_chemical_name_mineral           Nickel
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.5508
_cell_length_b                   3.5508
_cell_length_c                   3.5508
_cell_formula_units_Z            4
_cell_volume                     44.769
_database_code_amcsd             0014994
_diffrn_ambient_temperature      876.15
_exptl_crystal_density_diffrn    8.708
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9013004
X-ray measurement of the thermal expansion of pure nickel Sample: at T = 608 C Note: film 615
Owen, E. A.; Yates, E. L.; Philosophical Magazine 21 (1936) 809–819; doi:

data_9013005
_publ_section_title
;
 X-ray measurement of the thermal expansion of pure nickel
 Sample: at T = 608 C
 Note: film 615
;
_journal_name_full               'Philosophical Magazine'
_journal_page_first              809
_journal_page_last               819
_journal_volume                  21
_journal_year                    1936
_chemical_compound_source        Synthetic
_chemical_formula_sum            Ni
_chemical_name_mineral           Nickel
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.5516
_cell_length_b                   3.5516
_cell_length_c                   3.5516
_cell_formula_units_Z            4
_cell_volume                     44.799
_database_code_amcsd             0014995
_diffrn_ambient_temperature      881.15
_exptl_crystal_density_diffrn    8.702
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9013005
The structures of orthorhombic and vitrous arsenic Locality: synthetic Note: known as arsenolamprite
Smith, P. M.; Leadbetter, A. J.; Apling, A. J.; Philosophical Magazine 31 (1975) 57–64; doi:10.1080/14786437508229285

data_9013006
_publ_section_title
;
 The structures of orthorhombic and vitrous arsenic
 Locality: synthetic
 Note: known as arsenolamprite
;
_journal_name_full               'Philosophical Magazine'
_journal_page_first              57
_journal_page_last               64
_journal_paper_doi               10.1080/14786437508229285
_journal_volume                  31
_journal_year                    1975
_chemical_formula_sum            As
_chemical_name_mineral           Arsenolamprite
_space_group_IT_number           64
_symmetry_space_group_name_Hall  '-B 2ab 2'
_symmetry_space_group_name_H-M   'B m a b'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.65
_cell_length_b                   4.47
_cell_length_c                   11.00
_cell_formula_units_Z            8
_cell_volume                     179.471
_exptl_crystal_density_diffrn    5.546
_cod_original_cell_volume        179.470
_cod_database_code               9013006
Existence of the hexagonal modification of nickel Locality: synthetic
Weik, H.; Hemenger, P.; Bulletin of the American Physical Society 10 (1965) 1140–1140; doi:

data_9013007
_publ_section_title
;
 Existence of the hexagonal modification of nickel
 Locality: synthetic
;
_journal_name_full               'Bulletin of the American Physical Society'
_journal_page_first              1140
_journal_page_last               1140
_journal_volume                  10
_journal_year                    1965
_chemical_formula_sum            Ni
_chemical_name_mineral           Nickel
_space_group_IT_number           194
_symmetry_space_group_name_Hall  '-P 6c 2c'
_symmetry_space_group_name_H-M   'P 63/m m c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   2.622
_cell_length_b                   2.622
_cell_length_c                   4.321
_cell_formula_units_Z            2
_cell_volume                     25.726
_cod_data_source_file            13125.cif
_cod_data_source_block           global
_cod_database_code               9013007
_database_code_amcsd 0012144
Metastable structures of liquid-quenched and vapour-quenched antimony films Note: liquid-quenched specimen
Akhtar, D.; Vankar, V. D.; Goel, T. C.; Chopra, K. L.; Journal of Materials Science 14 (1979) 988–994; doi:

data_9013008
_publ_section_title
;
 Metastable structures of liquid-quenched and vapour-quenched antimony films
 Note: liquid-quenched specimen
;
_journal_name_full               'Journal of Materials Science'
_journal_page_first              988
_journal_page_last               994
_journal_volume                  14
_journal_year                    1979
_chemical_compound_source        Synthetic
_chemical_formula_sum            Sb
_chemical_name_mineral           Antimony
_space_group_IT_number           221
_symmetry_space_group_name_Hall  '-P 4 2 3'
_symmetry_space_group_name_H-M   'P m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.16
_cell_length_b                   3.16
_cell_length_c                   3.16
_cell_formula_units_Z            1
_cell_volume                     31.554
_database_code_amcsd             0013080
_exptl_crystal_density_diffrn    6.407
_cod_original_sg_symbol_H-M      'P m 3 m'
_cod_database_code               9013008
Metastable structures of liquid-quenched and vapour-quenched antimony films Locality: synthetic Note: liquid-quenched specimen
Akhtar, D.; Vankar, V. D.; Goel, T. C.; Chopra, K. L.; Journal of Materials Science 14 (1979) 988–994; doi:

data_9013009
_publ_section_title
;
 Metastable structures of liquid-quenched and vapour-quenched antimony films
 Locality: synthetic
 Note: liquid-quenched specimen
;
_journal_name_full               'Journal of Materials Science'
_journal_page_first              988
_journal_page_last               994
_journal_volume                  14
_journal_year                    1979
_chemical_formula_sum            Sb
_chemical_name_mineral           Antimony
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.61
_cell_length_b                   4.61
_cell_length_c                   4.61
_cell_formula_units_Z            4
_cell_volume                     97.972
_exptl_crystal_density_diffrn    8.254
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9013009
_database_code_amcsd 0013081
Metastable structures of liquid-quenched and vapour-quenched antimony films Note: liquid-quenched specimen
Akhtar, D.; Vankar, V. D.; Goel, T. C.; Chopra, K. L.; Journal of Materials Science 14 (1979) 988–994; doi:

data_9013010
_publ_section_title
;
 Metastable structures of liquid-quenched and vapour-quenched antimony films
 Note: liquid-quenched specimen
;
_journal_name_full               'Journal of Materials Science'
_journal_page_first              988
_journal_page_last               994
_journal_volume                  14
_journal_year                    1979
_chemical_compound_source        Synthetic
_chemical_formula_sum            Sb
_chemical_name_mineral           Antimony
_space_group_IT_number           139
_symmetry_space_group_name_Hall  '-I 4 2'
_symmetry_space_group_name_H-M   'I 4/m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.01
_cell_length_b                   3.01
_cell_length_c                   4.96
_cell_formula_units_Z            2
_cell_volume                     44.938
_database_code_amcsd             0013082
_exptl_crystal_density_diffrn    8.998
_cod_database_code               9013010
Metastable structures of liquid-quenched and vapour-quenched antimony films Locality: synthetic Note: liquid-quenched specimen Note: HCP structure resulted from electron beam heating of the tetragonal, FCC and SC structures
Akhtar, D.; Vankar, V. D.; Goel, T. C.; Chopra, K. L.; Journal of Materials Science 14 (1979) 988–994; doi:

data_9013011
_publ_section_title
;
 Metastable structures of liquid-quenched and vapour-quenched antimony films
 Locality: synthetic
 Note: liquid-quenched specimen
 Note: HCP structure resulted from electron beam heating of
 the tetragonal, FCC and SC structures
;
_journal_name_full               'Journal of Materials Science'
_journal_page_first              988
_journal_page_last               994
_journal_volume                  14
_journal_year                    1979
_chemical_formula_sum            Sb
_chemical_name_mineral           Antimony
_space_group_IT_number           194
_symmetry_space_group_name_Hall  '-P 6c 2c'
_symmetry_space_group_name_H-M   'P 63/m m c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   3.33
_cell_length_b                   3.33
_cell_length_c                   5.23
_cell_formula_units_Z            2
_cell_volume                     50.225
_exptl_crystal_density_diffrn    8.051
_cod_database_code               9013011
_database_code_amcsd 0013083
Metastable structures of liquid-quenched and vapour-quenched antimony films Locality: synthetic Sample: at room T Note: vapour-quenched specimen
Akhtar, D.; Vankar, V. D.; Goel, T. C.; Chopra, K. L.; Journal of Materials Science 14 (1979) 988–994; doi:

data_9013012
_publ_section_title
;
 Metastable structures of liquid-quenched and vapour-quenched antimony films
 Locality: synthetic
 Sample: at room T
 Note: vapour-quenched specimen
;
_journal_name_full               'Journal of Materials Science'
_journal_page_first              988
_journal_page_last               994
_journal_volume                  14
_journal_year                    1979
_chemical_formula_sum            Sb
_chemical_name_mineral           Antimony
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.61
_cell_length_b                   4.61
_cell_length_c                   4.61
_cell_formula_units_Z            4
_cell_volume                     97.972
_exptl_crystal_density_diffrn    8.254
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9013012
_cod_duplicate_entry 9013009
Metastable structures of liquid-quenched and vapour-quenched antimony films Locality: synthetic Note: vapour-quenched specimen Note: HCP structure resulted from electron beam heating of FCC structure
Akhtar, D.; Vankar, V. D.; Goel, T. C.; Chopra, K. L.; Journal of Materials Science 14 (1979) 988–994; doi:

data_9013013
_publ_section_title
;
 Metastable structures of liquid-quenched and vapour-quenched antimony films
 Locality: synthetic
 Note: vapour-quenched specimen
 Note: HCP structure resulted from electron beam heating of FCC structure
;
_journal_name_full               'Journal of Materials Science'
_journal_page_first              988
_journal_page_last               994
_journal_volume                  14
_journal_year                    1979
_chemical_formula_sum            Sb
_chemical_name_mineral           Antimony
_space_group_IT_number           194
_symmetry_space_group_name_Hall  '-P 6c 2c'
_symmetry_space_group_name_H-M   'P 63/m m c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   3.33
_cell_length_b                   3.33
_cell_length_c                   5.23
_cell_formula_units_Z            2
_cell_volume                     50.225
_exptl_crystal_density_diffrn    8.051
_cod_database_code               9013013
_cod_duplicate_entry 9013011
High-temperature thermal expansion of six metallic elements measured by dilatation method and X-ray diffraction Sample: at T = 293 K
Suh, I.-K.; Ohta, H.; Waseda, Y.; Journal of Materials Science 23 (1988) 757–760; doi:10.1007/BF01174717

data_9013014
_publ_section_title
;
 High-temperature thermal expansion of six metallic elements measured
 by dilatation method and X-ray diffraction
 Sample: at T = 293 K
;
_journal_name_full               'Journal of Materials Science'
_journal_page_first              757
_journal_page_last               760
_journal_paper_doi               10.1007/BF01174717
_journal_volume                  23
_journal_year                    1988
_chemical_compound_source        Synthetic
_chemical_formula_sum            Cu
_chemical_name_mineral           Copper
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.613
_cell_length_b                   3.613
_cell_length_c                   3.613
_cell_formula_units_Z            4
_cell_volume                     47.163
_database_code_amcsd             0013087
_diffrn_ambient_temperature      293
_exptl_crystal_density_diffrn    8.949
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9013014